en vue de l’obtention du
DOCTORAT DE L’UNIVERSITÉ DE TOULOUSE
Délivré par :
Université Toulouse 3 Paul Sabatier (UT3 Paul Sabatier)
Soutenue le mercredi 22 juin 2016
Optimization of the elaboration of insulating layers for the gate
structures and the passivation of MIS-HEMT transistors on GaN
(Optimisation de l'élaboration de couches isolantes pour les structures de
grille et la passivation de transistor MIS-HEMTs sur matériau GaN)
Directeurs de thèse :
M. Frédéric MORANCHO – Professeur des Universités, Université Toulouse 3 M. Alphonse TORRES – Ingénieur CEA-LETI
Membres du Jury
M. Yvon CORDIER Directeur de Recherche CNRS, CNRS-CRHEA Rapporteur
Mme Marie-Paule BESLAND Directrice de Recherche CNRS, IMN Jean Rouxel Rapporteur
M. Farid MEDJDOUB Chargé de Recherche CNRS, IEMN Examinateur
M. Gaëtan TOULON Ingénieur, EXAGAN Examinateur
M. Alain CAZARRÉ Professeur des Universités, Université Toulouse 3 Examinateur
Table of contents
General Introduction iii
1 GaN for power electronics : state of the art and context 1
1.1 Power electronics and devices . . . 1
1.1.1 Needs and demands of the market, specifications, theory VS reality . . . 1
1.1.2 Limits of silicon . . . 3
1.1.3 Wide band gap materials . . . 5
1.1.4 Figures of merit of semiconductors for power application . . 9
1.2 Place of GaN in power electronics . . . 11
1.2.1 Generalities on GaN and crystal structure . . . 12
1.2.2 GaN properties . . . 13
126.96.36.199 Electric properties . . . 13
188.8.131.52 Physico-chemical properties . . . 18
1.2.3 The AlGaN/GaN heterostructure . . . 19
184.108.40.206 Spontaneous and piezoelectric polarization . . . 21
220.127.116.11 Bidimensional electron channel . . . 23
1.2.4 Models and formation mechanisms . . . 26
1.3 Context of Ph.D. . . 31
1.4 Conclusion . . . 33
2 The Metal Insulator Semiconductor structure on GaN 35 2.1 Presentation of the structure . . . 35
2.1.1 Principle of operation. . . 35
2.1.2 The metal-semiconductor junction. . . 37
18.104.22.168 Full depletion approximation . . . 37
22.214.171.124 Full depletion analysis . . . 38
2.1.3 HEMT and MIS-HEMT threshold voltage . . . 41
2.2 Dielectrics on GaN and AlGaN . . . 45
2.2.1 MIS on GaN and AlGaN . . . 46
2.2.2 Surface contamination and interface states density. . . 48
2.3 Gate recess etching . . . 50
2.3.1 Principle . . . 50
2.3.2 Threshold voltage increase . . . 51
2.4 Conclusion . . . 52
3 Device realization 55 3.1 Origin and characteristics of the material . . . 55
3.2 Surface conditioning . . . 57
3.2.1 Chemical treatments . . . 57
3.2.2 Plasma treatments . . . 58
3.3 MIS-HEMT and capacitance fabrication . . . 59
3.3.1 Process flow . . . 60
3.3.2 Encountered difficulties and adopted solutions . . . 61
3.3.3 MESA etching insulation . . . 63
3.3.4 Metallization and ohmic contact . . . 63
3.3.5 High-κ dielectric deposition and in-situ N2 plasma treatment 64 3.3.6 Gate metal deposition . . . 65
3.4 Optional process : recess etching below gate . . . 66
3.5 Conclusion . . . 67
4 Results and discussions 69 4.1 Surface treatments and their characterization . . . 69
4.1.1 X-Ray Photo-electron Spectroscopy . . . 70
126.96.36.199 Principle . . . 70
188.8.131.52 Application to the AlGaN surface . . . 73
TABLE OF CONTENTS 3
184.108.40.206 HCl and SC2 treatments . . . 74
220.127.116.11 NH4OH and SC1 . . . 77
4.1.3 Plasma treatments . . . 81
18.104.22.168 Oxygen plasma . . . 81
22.214.171.124 Nitrogen containing plasma . . . 81
4.1.4 Surface treatments conclusion . . . 84
4.2 Schottky gate devices . . . 85
4.2.1 C(V) results . . . 85
4.3 MIS structures . . . 88
4.3.1 Thermal ALD structures . . . 88
126.96.36.199 C(V) results. . . 88
188.8.131.52 Id(Vg) results on circular transistor with Lg=100µm 91 4.3.2 PEALD structures . . . 93
184.108.40.206 C(V) results. . . 93
220.127.116.11 Id(Vg) results on circular transistor with Lg=100µm 99 4.4 Influence of the dielectric thickness . . . 101
4.4.1 C(V) results . . . 102
4.4.2 Id(Vg) results on circular transistor with Lg=100µm . . . 103
4.4.3 Threshold voltage evolution . . . 105
4.5 Influence of post-deposition thermal treatment . . . 106
4.5.1 C(V) results . . . 107
4.5.2 Id(Vg) results on circular transistor with Lg=100µm . . . 109
4.6 Superiority of PEALD over thermal ALD . . . 111
4.7 Normally-Off architecture : MIS structure with partial or full AlGaN recess etching . . . 119
4.7.1 Gate Recess Etching . . . 119
18.104.22.168 C(V) Results . . . 119
22.214.171.124 Id(Vg) results on circular transistor with Lg=100µm122 126.96.36.199 Threshold voltage evolution . . . 124
4.7.2 AlGaN Full-recess etching below gate . . . 125
4.8 Conclusion . . . 127
First and foremost I would like to thank the CEA-Leti and the LAAS-CNRS for allowing me to do my PhD under their care and supervision. I would like espe-cially to thank the LC2E laboratory and all its members in CEA-Leti, where I had the chance to do the entirety of my thesis under the supervision of Mr. Alphonse TORRES. Regarding LAAS-CNRS, I would like to thank the professor and su-pervisor of my work, Pr. Frédéric MORANCHO who supported me continuously during all my research. It was a great pleasure and privilege to work with all these competent and kind scientists and researchers.
Still in CEA-Leti, I would like to acknowledge the PTA (Plateforme de Tech-nologie Amont) and the CIME (Centre Interuniversitaire de MicroElectrnoique), which offered me the possibility and necessary formations to work on their equip-ment. A special thanks goes to all the members of those two clean rooms which assisted me during my PhD and provided with invaluable knowledge, help and advice.
I would also like to thank the III-V Lab which provided me with some very good quality material and services, which greatly contributed to the success of my work and my obtaining great results.
This section could not be complete without thanking Dr. Yvon CORDIER and Dr. Marie-Paule BESLAND which agreed to be my reviewers, and were very kind and comprehensive all throughout the correction process. Acknowledgments go as
well to the other members of my jury, Mr. Farid MEDJOUB and Mr. Gaëtan TOULON, and its president Pr. Alain CAZARRÉ.
Last but not least, a special thanks goes to my family, friends and CEA co-PhD students who supported, encouraged and assisted me all along my PhD research. They have been a tremendous support during those years, and I consider myself very lucky to have them in my life. The last word goes to my companion, Julie RANDRIANARISOA, without whom I could never have come as far as I am now. Her love and infallible support is greatly responsible for me completing this PhD, and I will always be grateful for her being at my side.
Throughout the 20thcentury, humanity has thrived like it never had before, mostly
through the use of fossil fuels and their derivatives. Whether it be for transporta-tion, energy production or synthetic products, most of the world and its industry as we know it now would not have been, and still could not be possible without the use of oil and gas. However, as we now entered the 21st century, we also realize
the dire impacts this had on our environment. Greenhouse gas levels have never been as high as they are now, and CO2 emission has become one if not the major
concern in ecology throughout the world. But despite the growing global aware-ness of the problem, energetic needs are constantly rising due to economic growth of emerging countries and world population growth, with International Energy Agency estimations predicting that electricity consumption throughout the world could rise by 75% in less than 25 years (according to Areva). And with the rapid decay of fossil fuels reserves, we could soon be confronted with one of the major challenges humanity has ever faced. As a consequence, innovation in the energy domain has become one of the main research focus this last years. The advent of solar and wind technology paved the way for new possibilities in terms of clean energy production, and hybrid or fully electrical technologies have recently made leaps in terms of performance and sustainability.
Parallel and directly linked to the development of those various "green" tech-nologies, energy conversion has now become one of the cornerstones for the
vement of electrical performances and consumption. As electronic devices become more and more complicated, energy conversion systems have multiplied and are often the guarantors of an optimal functioning. Generally referred to as power electronics, they are most of the time constituted of semiconductors like power transistors, which can in turn be directly linked to losses in circuits. With more than 10% of the produced energy being lost in the conversion process , improving those systems has become mandatory for a better, cleverer and more economical way of managing energy.
Largely dominated by silicon based components, the semiconductor industry is now gradually faced with a growing need for evolution, particularly in the power industry. While they have greatly contributed towards circuits performance optimi-zation, Si based technologies are now arriving at maturity and their further growth has become limited by the intrinsic properties of the material. As such, it becomes necessary for a new generation of components to appear in order to push back the limits defined by actual technology. As such, large band gap material appear as one of the go-to solutions, their physical properties largely surpassing the ones of silicon or this particular application. Recent years studies have notably been marked by the arrival of incredible like gallium nitride GaN and silicon carbide SiC. Furthermore, recent developments in heteroepitaxy of GaN on Si allowed to combine the efficiency of improved performance with low cost production on large scale wafers (200 mm). It thus marked a real rupture with silicon components and became a very serious candidate for future generations of power converters.
However, despite its appealing properties and general scientific consensus on its potential, GaN on Si technology is still being confronted with many challenges that hinder its developments and slows its market introduction. This is particularly true for high bias (>1000 V) and high current (> 100 A) applications where quality of the material and robustness of technology are primordial. It is precisely in this context that this Ph.D. is inscribed, through the study and development of one of the key technological steps that comes into play for the fabrication of a
HEMT (Metal Insulator Semiconductor - High Electron Mobility Transistor). The present work will be mostly focused on the insulating step of the process, with the main objective of improving the electrical behavior of the transistor through gate leakage reduction while reducing interface states density. This manuscript is the culmination of three years of studies and experimentation and is divided in four chapters.
Chapter 1 : This chapter will first focus on describing the properties of a power converter should have in order for them to respond to the needs and demands of the current market, and highlight why there is a need for wide band gap materials in today’s industry. It will then assess the place of GaN in power electronics through the study of its properties, and expose the reasons why it is becoming a key player.
Chapter 2 : Focused on the Metal Insulating Semiconductor on GaN, this se-cond chapter will review the different equations responsible for the unique and peculiar behavior of transistors made on an AlGaN/GaN heterostructures. As it is the main subject of the present study, the major focus will then be on the in-troduction of the insulating layer and the impact it will have on the MIS-HEMT’s electrical properties. Also, and though it was at first not intended to be realized during this Ph.D., the influence of the gate recess etching on the threshold voltage increase will also be described in the last part of the chapter.
Chapter 3 : This chapter will describe all the different technological steps I put in place and performed during my Ph.D. First, I will describe the surface condi-tioning processes that were studied. In a second time, I will expose all the process flow that was used in order to achieve the completion of functional MIS-HEMT structures, through the creation of diodes and circular transistors in particular. Lastly, I will detail the optional process of recess etching below the gate that I could implement inside the devices’ elaboration
Chapter 4 : This final chapter will be the heart of the present study, where the results of my work will be presented and commented upon. In a first part, surface treatments and their characterization will be the main topic, with an emphasis on the results obtained through X-ray Photo-electron Spectroscopy. The rest of the chapter will then review all the electrical results that were obtained through the study of Schottky gate devices and fully functional MIS-HEMT structures. Capacitance C(V) and gate current Id(Vg) measurements will be at the center of
those results. They will assess the impact of the insulating layer deposition method, how results evolve depending on its thickness, and how post deposition thermal treatment might have an influence. Last but not least, I will present how a partial or full gate recess etching impacted electrical properties and helped to achieve a normally-off architecture.
GaN for power electronics : state of the
art and context
Power electronics and devices
Needs and demands of the market, specifications,
theory VS reality
The ever growing demand of energy is one of tomorrow’s greatest challenge if we want to keep the standards as they are today. Despite our efforts, the demand for electricity keeps to increase, and is expected to do so more than any other resources in future years. With a growth of 2.5% each year, levels of demand and
production of electricity should be twice as large in 2013 as they were in 2006. The technology using power electronics is the key to regulating energy flux between the power source and the devices. In every system needing electricity to operate, it is responsible for reliability, stability and efficiency of the way in which the energy is spent. And whether it be for personal computers and domestic appliances, or for transportation and heavy industry, global semiconductor market in this particular domain is accountable for more than 50 billions of dollars in 2010 alone. Optimization of power management requires components able to sustain high voltage and current levels, at high frequencies and high temperature, with low losses in conduction as well as commutation.
Power electronics is the technology that concerns energy conversion. With less than 50 years of existence, it still is a young technology but has known a great and rapid development in recent years, due to the fact that more than 15% of produced electrical energy needs some kind of conversion. It is a technology that is based on commutation electronics, and takes advantage of the properties of a perfect switch : it does not dissipate any energy, whether it is perfectly closed (null resis-tance, no bias between source and drain) or perfectly opened (infinite resisresis-tance, no current going through). When associated with different filtering elements, it is thus theoretically possible to modify voltage and/or current, without any losses. Unfortunately, reality does not match theory yet and losses are still unavoidable because of the physical components which are part of power switches. However, the increasing efficiency in the devices and the overall size, weight and cost re-duction allowed the generalization of power electronics components in domains where losses must be kept to a minimum, in order to reduce heating and achieve high yield performances. The automotive market is a perfect example where such technology will play a key role in future developments. In the coming 20 years, it is expected that cars will evolve from fully thermal to fully electric while going through intermediate hybrid states. The energy management in these new kind of engines is becoming more and more challenging and will require sophisticated
elec-1.1. POWER ELECTRONICS AND DEVICES 3
tronic modules such as power converters in order to sustain optimum functioning regimes.
Limits of silicon
Today, silicon is the core material used in most semiconductor technologies. It is at the foundation of modern electronics as we know them and can be found in a large majority of components. But with the rapidly increasing demand in power electronics, the microelectronics industry is now confronted with the intrinsic limits of silicon.
As stated earlier, power components play the role of switches with two different states :
- an on-state, where specific resistance RON must be as low as possible. We
sometimes use RON· S, S being the active surface of the power component, in
order to introduce a notion of volume and cost.
- an off-state, where the voltage withstand must be as high as possible until breakdown voltage VBD is reached.
Both characteristics are closely related to the lowly doped layer (epitaxial layer in most cases), which plays a double role : it ensures the voltage withstand in the off-state, and has an important resistive effect in the on-state. We thus have the following relation :
RON· S(Ω · cm2) = α · V β
where α and β are two positive and real constants. This equation defines the limits of silicon : the value of the specific on-state resistance cannot be inferior to a value related to the bias we want the power component to sustain.
If we look at figure 1.1, we can see the silicon limits and how they fare compa-ratively to large band gap materials and different architectures.
Figure 1.1 – Specific chip resistance Ron in function of rated switch voltage for
We can see that there is a large zone where silicon components cannot grant the needed characteristics, even with complex architectures such as IGBTs for ins-tance. And if we want to comply with the power increase, it has become necessary in silicon technology to increase the size of the components. However, this does not represent a viable solution since the size increase will lead to higher energy losses, especially in commutation, and that does not agree with the current mar-ket tendency where size reduction and high energy efficiency are of the utmost importance. It is thus capital to develop a new and innovative technology based on compatible materials for us to overcome those limitations.
1.1. POWER ELECTRONICS AND DEVICES 5
Wide band gap materials
In this context where silicon is no longer an option, the emergence of wide band gap materials is regarded as the most promising solution in the power electronics industry. With operating constraints such as high temperatures (300-700 K) and high voltage (> 600 V), silicon carbide (SiC), gallium nitride (GaN) and diamond are the most promising candidates to date. Compared to silicon, they present the advantage of working on a large scale of temperatures, a high breakdown electric field and a high electron saturation velocity.
Having a large band gap (around 3 eV) will reduce the thermoionic carrier formation, which, if to high, can change the nature of the semiconductor. Those carriers are formed following an Arrhenius law, n = n0e−Ea/kT, where Ea is the
activation energy, k the Boltzmann constant and T the temperature. In the case of semiconductors, the activation energy is the gap energy Eg. This explains why
large band gap materials are preferable for high temperature uses, since the higher Eg will be, the lower the influence of temperature becomes.
And furthermore, critical breakdown field in semi-conductor materials is di-rectly related to their band gap energy [2, 3]. So the higher the band gap, the higher the breakdown field is, which allows these materials to have exceptional voltage withstands.
Table 1.1 shows the main electrical characteristics of conventional and wide band gap semiconductors.
Conventional Large band gap
Silicon GaAs 6H-SiC 4H-SiC GaN
Dia-mond Gap energy Eg (eV) 1.12 1.43 3.03 3.26 3.39 5.45 Electron mobility µn (cm2· V−1· s−1) 1450 6500 850 980 1250 2000 Hole mobility µp (cm2· V−1· s−1) 450 400 101 115 35 2000 Critical breakdown field Ec (MV · cm−1) 0.3 0.4 2.5 3 3.3 10 Intrinsic carrier density ni (cm−3) 1.×1010 2.×106 2.×10−6 8.×10−9 1.×10−10 1.×10−27 Thermal conductivity λ (W · cm−1· K−1) 1.412 0.455 4.9 4.9 1.3 20 Relative permitivity r 11.8 13.1 9.66 10.1 9.5 5.7 Electron saturation velocity νsat (×107 cm · s−1) 1 1 2 2 2.2 2.7
Table 1.1 – Electrical properties of conventional and wide band gap semiconduc-tors.
Of all the different materials, diamond exhibits the best overall properties for power applications, followed by gallium nitride which is also a good candidate for optoelectronics and power due to its direct gap and its breakdown electric field 10 times that of silicon. However, it has the smallest thermal conductivity, compared
1.1. POWER ELECTRONICS AND DEVICES 7
to the other materials.
With three different crystalline structures available, silicon carbide is also a good candidate for power electronics. With an hexagonal atomic structure, 4H-SiC and 6H-4H-SiC are only differing by their mobility which is isotropic in the first and super to the anysotropic one in the last. 3C-SiC has the highest electron mobility and saturation velocity because of reduced phonon scattering resulting from the higher symmetry of its cubic atomic structure.
All those materials have a higher breakdown field compared to silicon and are able to sustain a voltage roughly 10 times superior. Consequently, for the same voltage withstand, a component made from wide band gap material can be made with a thickness 10 times inferior, or with a doping a 100 times higher in the drift section (lowly doped layer) than that of a typical PN− junction. For this typical kind of junction, the breakdown voltage is directly related to the critical breakdown electric field following this relation :
VBD(V ) =
0· r· Ec2
2 · q · Nd
(1.2) where 0 and r are respectively the void and the semiconductor permittivity, q is
the electron elementary charge, Nd the doping level in the N− region and Ec the
critical breakdown field.
Specific on resistance can be given by this equation  :
RON· S(Ω · cm2) =
27 · V2
8 · 0· r· µn· Ec2
(1.3) where µn is the electron mobility.
8 1. GAN FOR POWER ELECTRONICS : STATE OF THE ART AND CONTEXT
If the power loss is determined by the first two terms can be used reasonably as a figure of merit (FOM) for MOSFETs.
If the gate drive circuit impedance is assumed to be is negligibly small, the 2nd term in Eq.(16) disappears. The switching loss is determined only by the main junction capacitance loss as
tion, the equality holds if the first and the second terms are equal to each other. . Again, if the small compared with the first is regarded reasonably as a new FOM, which is discussed in detail in the next Section.
㻣 㻡 㻤 㻜 㻤 㻡 㻥 㻜 㻥 㻡 㻝 㻜 㻜 㻜 㻡 㻝 㻜 㻝 㻡 㻞 㻜 㻞 㻡 㻟 㻜 㻟 㻡 㻵㼛㼡㼠 㻔 㻭 㻕 㻱 㼒 㼒 㼕 㼏 㼕 㼑 㼚 㼏 㼥 㻌 㻔 㻑 㻕 㼂㼕 㼚 㻦 㻝 㻞 㼂㻘 㻌㼂㼓 㻦 㻡 㼂㻘 㼂㼛 㼡 㼠 㻦 㻝 㻚 㻟 㼂㻘 㼒㼟 㼣㻦 㻝 㻹 㻴㼦 㻿 㼕 㻌 㼘 㼕 㼙 㼕 㼠 㻾 㻳㻩 㻜 㻚 㻠: 㻾 㻳㻩 㻟 㻚 㻣: : : :
Fig.17 RonQstr as function of breakdown voltage
H HP P
Breakdown Voltage [V]1 1 0 1 e 2 1 e 3 1 e 4 1 e 5 1 e 6
]Ga NL im it SiC Lim it Si Lim it 10 100 1䡇V 10䡇V IGB T IGB T SJM OS SiC MO S GaN GaN FET FET 30VMOSFET
Breakdown Voltage [V]1 1 0 1 e 2 1 e 3 1 e 4 1 e 5 1 e 6
]Ga NL im it SiC Lim it Si Lim it 10 100 1䡇V 10䡇V IGB T IGB T SJM OS SiC MO S GaN GaN FET FET 30VMOSFET
Figure 1.2 – Ron versus breakdown voltage for Si, SiC and GaN, with their
For a unipolar component presenting specific on-resistance below 1 Ω · cm2,
limits of silicon is around 1 kV whereas wide band gap semiconductors allow the fabrication of components able to sustain more than 10 kV. For advanced power applications, only those materials are able to cope with the needed specifications as can be seen in figure 1.1).
Again, diamond is the material presenting the best electrical and thermal pro-perties. With its low intrinsic carrier concentration, it is thus able to sustain high temperatures. However, its fabrication process is still at an early stage and condi-tions to achieve the production of diamond are still hard to meet. Furthermore, if we limit ourselves to the previous equations, we do not take into account techno-logical aspects which can have an important role, such as changing the mobility through the use of doping, which is a very difficult process to implement in dia-mond.
Compared to diamond and GaN, SiC is the material presenting the most ad-vanced technology, with actual power devices being commercialized. The JFET on
1.1. POWER ELECTRONICS AND DEVICES 9
SiC transistor is right now the most advanced power switch, being able to perform at temperatures up to 300 ◦C. However, the high price of large SiC diameter sub-strates and associated epitaxies (around a 100 times higher than silicon) makes it a debatable solution in terms of economical concerns.
Figures of merit of semiconductors for power
In order to compare the possible power electonics performance of different mate-rials, some commonly known figure of merit are liste in Table 1.2. The numbers in this table have been normalized in repect to Si, and le larger the number, the better the material’s performance in the corresponding category. We can notice that SiC polytypes and GaN have similar figures of merit, which implies similar performances. Diamond’s figure of merit are at least 40 to 50 times more than any other semiconductor in the table.
Material Si GaAs 6H-SIC 4H-SiC GaN Diamond
JFM 1.0 1.8 277.8 215.1 215.1 81,000 BFM 1.0 14.8 125.3 223.1 186.7 25,106 FSFM 1.0 11.4 30.5 61.2 65.0 3,595 BSFM 1.0 1.6 13.1 12.9 52.5 2,402 FPFM 1.0 3.6 48.3 56.0 30.4 1,476 FTFM 1.0 40.7 1470.5 3424.8 1973.6 5,304,459 BPFM 1.0 0.9 57.3 35.4 10.7 594 BTFM 1.0 1.4 748.9 458.1 560.5 1,246,711
Table 1.2 – Main figure of merit for wide bandgap semiconductors compared with Si 
JFM Johnson’s figure of merit is a measure of the ultimate high frequency ca-pability of the material. More specifically, it is the product of the charge carrier saturation velocity in the material and the electric breakdown field under same conditions, first proposed by A. Johnson of RCA in 1965.
J F M = vsatEBD
where vsat is the saturation velocity and EBD is the electric field at which impact
ionization initiates breakdown. Unfortunately, this figure of merit is difficult to determine experimentally as both vsat and EBD are intrinsic properties of a device,
although easily found from simulation.
BFM Baliga’s figure of merit is a measure of the specific on-resistance of the drift region of a vertical FET . The BFM is useful in order to compare different semiconductor materials in high power voltage applications. It takes into account the barriers mobility and the dielectric permittivity of the material, as well as its critical electric field. It is expressed as :
BF M = εrµnEc3 (1.5)
It is mainly used for low frequency applications where conduction losses are predominant. It gives an appreciation in terms of voltage sustaining capability.
FSFM This is the FET switching speed figure of merit.
BSFM This is the bipolar switching speed figure of merit.
FPFM This is the FET power handling capacity figure of merit.
1.2. PLACE OF GAN IN POWER ELECTRONICS 11
BPFM This is the bipolar power handling capacity figure of merit.
BTFM This is the bipolar switching product figure of merit.
Place of GaN in power electronics
Gallium was discovered in 1875 in France by Lecoq de Boisbaudran through the spectroscopy analysis of the zincblende from Pierrefitte in the French Pyrénées. Discovered around 1920, gallium nitride GaN crystal was first studied in the seven-ties but was then abandoned due to synthesis difficulseven-ties. In the nineseven-ties, under the influence of Japanese research groups, great progress was achieved in synthesizing the crystal. In 1997 and 2000, the development of a new prototype of MBE (mole-cular beam epitaxy) for Research and Development (R&D) allowed to grow nitride materials such as GaN. Because of its direct gap, it was first used for optoelec-tronic devices. Later on, its mobility and its high electron saturation velocity was used for designing HEMT (high electron mobility transistors) structures for high frequency (HF) application, and high temperature and high voltage applications were possible thanks to its high breakdown field. Until then, difficulties with high levels of P doping, resulting in device resistance being too important, represented a great challenge for HF bipolar technologies. However, work is still under progress in order to solve the inherent problems associated with technological process :
- GaN does not exist in liquid phase, which makes it difficult to obtain bulk GaN substrates. To date, epitaxy is realized on sapphire, silicon carbide or silicon substrates through metal organic chemical vapor deposition (MOCVD) in order to reduce fabrication costs. The choice of the substrate is based on a compromise between price, performances and device reliability ;
- thermal oxidation, which is largely used in the silicon MOS and CMOS in-dustry, is not possible on GaN due to the poor quality of the native oxide ;
- despite the fact that it is now possible to produce high quality material on 200 mm silicon substrates, defect density remains very high ;
Nowadays, silicon IGBTs and thyristors are the only available options for high voltage applications (1 - 10 kV), but it is expected that GaN unipolar components (HEMTs and MOSFETs) could replace those devices. This could lead to higher frequencies, higher voltages and higher temperatures of operation. However, GaN thermal conductivity is relatively low which poses problems to evacuate heat during conception of the devices. Nonetheless, it remains much cheaper than diamond and far more adapted to doping.
Generalities on GaN and crystal structure
Gallium nitride (GaN) is part of the nitride III-N family which is composed of boron-nitride (BN), aluminum-nitride (AlN) and indium-nitride (InN). They can crystallize under a cubic or hexagonal form, but the hexagonal phase is the most stable we can achieve through standard growing conditions. Those two structures are zinc blende (cubic) and wurtzite (hexagonal) which can be seen in figure1.3.
Figure 1-1b : structure zinc blende. Figure 1-1a : structure Wurtzite.
Figure 1.3 – GaN cubic Zinc Blende (left) and hexagonal Wurtzite (right) struc-ture.
The latter is the one being used in laboratory for GaN layers epitaxy due to its metastable nature, which presents numerous crystalline properties suitable to the elaboration of heterojunctions. Table1.3 shows the crystal parameters of both structures.
1.2. PLACE OF GAN IN POWER ELECTRONICS 13
Cubic c-GaN Hexagonal h-GaN
Lattice parameter a300K = 4.511Å
a300K = 3.188Å
a300K = 5.185Å
Table 1.3 – Lattice parameters for GaN crystalline structures.
The c/a ratio of the GaN lattice is very close to the q8/3 theoretical value for a perfect hexagonal structure. We can thus assume that gallium atoms are in lowly distorted tetrahedral sites.
188.8.131.52 Electric properties
GaN is a semiconductor presenting a direct band gap, which means that the conduction band minimum (Ec) and the valence band maximum (Ev) are at an
almost identical value on the diagram representing the energy E relatively to the wave vector k. For GaN, this point is located at the Γ point, center of the Brillouin zone (k = 0). The first Brillouin zones and the band structures in the major di-rection are represented in figure 1.4.
Figure 1.4 – GaN cubic Zinc Blende (left) and hexagonal Wurtzite (right) struc-ture and their Brillouin zones.
Hexagonal and cubic structures have a band gap of 3.43 eV and 3.20 eV respec-tively at 300 K. Those values rise with temperatures, as described in the following equation :
Eg = E0 −
a · T2
T + b (1.6)
where E0 = 3.47 eV, a = 0.599 meV.K−1 and b = 880 K. This formula gives us a
gap of 3.424 eV for hexagonal GaN at a 300 K temperature. This energy is to be compared to the 4H-SiC value of 3.240 eV and the Si value of 1.103 eV at 300 K obtained through the same calculation. This band gap energy is directly related to the breakdown field, which we will take into account later on. A wide band gap is generally associated to a low intrinsic carrier concentration, but non intentionally doped GaN is always n-type doped and electronic density can vary from 1016
to 1019 at.cm−3 depending on the growing conditions. However those values are
not very accurate since defects in the GaN structure will contribute to obtain higher values, while compensation phenomenons, located at deep energy levels, can contribute to the general lowering of these values. Hall measurements allow more precise and reliable way to obtain accurate values for the density and donor activation energy depending on temperature. The activation energy is related to the carrier concentration and given by the following equation :
Ea(Nd) = Ea(Nd= 0) − δ · Nd1/3 (1.7)
where δ is the shield constant in GaN (2.4x10−8 eV.cm−1). For a doping level of 3x1017 at.cm−3, we have an activation energy of 17 meV. Beyond 3x1018 at.cm−3,
activation energy becomes null and electronic density does not decrease with tem-perature, which corresponds to a metallic behavior (semiconductor beyond the Mott transition).
As stated earlier, another very important characteristic in power electronics is the breakdown electric field since this parameter will directly influence the
maxi-1.2. PLACE OF GAN IN POWER ELECTRONICS 15
mum bias sustainable by the component. The higher its value, the easier it will be to elaborate devices with high doping levels and reduced size, with the beneficial properties such as a lower on-resistance. The theoretical breakdown field in GaN is compared to the one of other semiconductors in figure 1.5
Eg (eV) à 300K 0 1 2 3 4 5 6 EC (1 0 6V. cm -1) 0 2 4 6 8 10 12 Gap indirect Gap direct Diamant GaN 4H-SiC 3C-SiC GaAs Si 6H-SiC
Figure I-3 : Champs critiques de différents matériaux
Figure 1.5 – Critical breakdown fields for different semiconducting materials with a doping concentration of 1016 cm−3 depending on their gap (at 300 K)
We can see that large band gap materials have superior breakdown field compa-red to materials such as silicon or gallium-arsenide. Diamond’s critical breakdown field (around 10 MV.cm−1 at 300 K) is theoretically a hundred times higher than
silicon’s, while at 3.4 MV.cm−1, gallium-nitride’s is eleven times higher.
As stated previously, breakdown electric field and bang gap energy are tightly related by the following formula :
EC ∝ Eg3/2 (1.8)
According to this relation, we can see that the higher the gap, the higher the theoretical breakdown field will be, as shown on figure 1.5. This also means that the critical field will decrease as temperature rises.
Last but not least of the electric parameters is the electron mobility. Under the influence of an electric field, charge carriers (electrons and holes) will migrate in the material, and the mean free path without interaction will set the movements of those carriers in the crystal. Generally wrote as µ, the mobility will be under the direct influence of any modifications in the lattice, such as those induced by temperature rising or doping. Those dependency can be calculated by the following formula : µ = µmin( T 300) β +µmax( T 300) α− µ min(300T )β 1 + (Ntot Nref) γ (1.9)
where T is the temperature, N the carrier concentration, α, β and γ parameters directly related to the semiconductor considered. Table 1.4 shows those values for GaN. Carriers µmin (cm2.V−1.s−1) µmax (cm2.V−1.s−1) Nref (cm−3) α β γ Electrons 55 1000 2x1017 -2 -3.8 1 Holes 30 170 3x1017 -5 -3.7 2
Table 1.4 – Minimum and maximum carrier mobility in GaN and associated calculation parameters .
If we now look at figure 1.6, we can trace the evolution of the electron and hole mobility for temperature ranging from 150 K to 475 K for different carrier concentration.
The first thing we can notice here is that mobility will decrease inversely pro-portional to the doping of the semiconductor. For a low concentration, we can also see that temperature has a large impact on mobility. For a carrier density around 1016cm−3, GaN mobility is around 900 cm2.V−1.s−1 at 300 K, which is very similar
to the one of 3C-SiC. However, hole mobility is around 170 cm2.V−1.s−1, which is 4 times more important than in 3C-SiC, but also 4 times lower than silicon’s.
1.2. PLACE OF GAN IN POWER ELECTRONICS 17 è Porteurs .s ) max (cm Electrons 1000 Trous 170 Concentration (cm-3)
1e+15 1e+16 1e+17 1e+18 1e+19 1e+20
M o b il ité ( cm 2.V -1 s-1) 200 400 600 800 1000 1200 1400 250K 275K 300K 325K 350K 375K 400K 425K 450K 475K (a) Porteurs .s ) .s ) (cm ) α β γ Electrons 2x10 -2 -3,8 1 Trous 3x10 -5 -3,7 2 Concentration (cm-3 )
1e+15 1e+16 1e+17 1e+18 1e+19 1e+20
M o b il ité ( cm 2.V -1.s -1) 100 200 300 400 500 250K 275K 300K 325K 350K 375K 400K 425K 450K 475K
Figure 1.6 – Electron (left) and hole (right) mobility depending on carrier concen-tration as calculated using equation 1.8.
Those values are reported in Table 1.5
Semiconductor Electron mobility (cm2.V−1.s−1) at 300K Hole mobility (cm2.V−1.s−1) at 300K GaN 900 170 3C-SiC 900 40 4H-siC 750 115 Si 1360 600 GaAs 8500 400
Table 1.5 – Carrier mobility in semiconductors at 300K.
The main difference between the mobility in GaAs and GaN is related to the difference in the effective mass of the carriers, which is higher in GaN, but this apparent superiority of GaAs over GaN is not valid anymore under a high electric field. In fact, III-V semiconductors band structure is peculiar and under those conditions, the variation of mobility is non-linear and not continuously increasing as is the case in other semiconductors. At 200 kV/cm for GaN, there is an over-speed peak which induces a higher electron velocity. As a consequence, saturation velocity is reached a lot later, which is why GaN can be used at high voltages.
184.108.40.206 Physico-chemical properties
One particular property of the GaN crystal, when growing along the 0001 direction (which is the most common) perpendicular to the c plane, is that it is polarized. And since the structure does not present any inversion center, (0001) and (0001) directions are not identical. In consequence, those two directions define different types of surface, which are the Ga(0001) face and the N(0001) face.
Associated to this macroscopic polarization comes a piezoelectric polarization. Though the origin and orientation of both polarizations are identical, the direction of the piezoelectric one changes depending on the strains in the epitaxial layer.
The electric field generated by the global polarity could be problematic for optoelectronic devices since the recombination of carriers in quantum wells will diminish, thus lowering the LEDs efficiency. However for FETs (Field Effect Tran-sistors) and HEMTs (High Electron Mobility TranTran-sistors) architectures, the high electric field will be highly beneficial, especially for the formation of a 2D electron gas on which we will come back later on. Regarding fabrication processes, the dif-ferent nature in the faces will influence the behavior of GaN regarding thermal treatments, cleanings or metal adherence during deposition.
Regarding thermal properties, GaN thermal conductivity is 1.3 W.K−1.cm−1 but depends on crystal quality. In a power electronics domain where large heat dissipation is necessary, it represents the capacity of the material to transfer a certain quantity of heat per time constant (1 W = 1 J.s−1) and per surface unity under a temperature gradient. Thermal conductivity of GaN is relatively close to the one of silicon (1.5 W.K−1.cm−1). It is however 3 times higher than GaAs and sapphire conductivity, but 3 to 4 times lower than SiC depending on the polytype. Ideally, this value has to be as high as possible for power electronics since non dissipated heat will generate a rise in the component temperature, which translates into a lowering of the mobility and thus of the global electric performances of the components.
infor-1.2. PLACE OF GAN IN POWER ELECTRONICS 19
mation on how the material will dilate or contract depending on the temperature. This is a parameter to keep in mind when choosing the base substrate material for growth during hetero-epitaxy. Table 1.6 gives the thermal values for different semiconductor materials.
Thermal conductivity Thermal dilatation coefficient (W.K−1.cm−1) (x10−6 K−1) ∆a/a 300K ∆a/a 900K h-GaN 1.3 5.59 5.11 Si 1.5 2.6 4.2 3C-SiC 4.9 3.8 4.8 GaAs 0.5 5.73 6
Table 1.6 – Theoretical values for thermal conductivity and thermal dilatation coefficient in semiconductors [9, 10,11].
The AlGaN/GaN heterostructure
As stated earlier, one of the major applications in power devices for which GaN is considered among the best materials, is the creation of HEMT structures. Compa-red to traditional MESFET (Modulation Electron Surface Field Effect Transistor), the HEMT is able to bypass the problem of electron transportation in highly doped environment, which presents many restrictive phenomenons regarding electronic performances, especially for mobility. The main principle behind the high mobility transistor is to create a bidimensional electron gas (2DEG) using an AlGaN/GaN heterojunction, which band diagram is represented in figure 1.7.
Figure 1.7 – Band diagram for the AlGaN/GaN heterostructure, with Ef the
Fermi level energy, EC the conduction band energy and ΦB the Schottky
bar-rier height. ∆EC is the energy difference between the AlGaN and GaN respective
conduction bands .
By choosing the right material, we can create a localized potential drop of the conduction band below the Fermi level and confine the carriers in a quantum well. The resulting potential and associated band diagram are thus directly related to the band gap of each semiconductor and their respective doping levels. The electron exchange between the two materials allow Fermi levels alignment and, as in a PN junction, a space charge appears.
The resulting well in GaN is a high electron density region with an excellent mobility, since it is free of any impurity. Electrons can move freely between source and drain along the heterojunction in a bidimensional space. Despite the restrictive aspect of the 2DEG, electron concentration in such structures can achieve very high levels, up to 2x1013 cm−2. It is important to notice that this value is referenced as a unit of surface and not volume.
1.2. PLACE OF GAN IN POWER ELECTRONICS 21
The HEMT structure represented in figure2.2presents a typical heterojunction between the GaN buffer layer and the AlGaN barrier. In this transistor, gate modulation is achieved by applying negative voltages which allows to deplete more or less the bidimensional channel between the gate and the drain. This kind of operation is referred to as depletion transistor or normally-on.
Source Gate Drain
Insulator AlGaN Barrier
2DEG GaN Buffer
Substrate (SiC or Si)
Figure 1.8 – Schematics of a typical AlGaN/GaN HEMT with and insulation layer.
220.127.116.11 Spontaneous and piezoelectric polarization
One of the specifications of the HEMT structure based on GaN is that there is no need to dope the barrier layer, in our case AlGaN, in order to obtain a high electron density in the potential well (as opposed to GaAs for example). Electric fields are indeed already present in the AlGaN/GaN heterojunction and they will allow the formation of a high density bidimensional electron gas. Those electric fields are the consequence of 2 types of polarization : spontaneous and piezoelectric polarization.
Spontaneous polarization Without being under the influence of any mecha-nical constraint, the crystalline structure of GaN presents a spontaneous
polariza-tion. It is the result of the non-superposition of the barycenters of the negative and positive charges in the crystal (electrons and holes respectively). It is also present in AlGaN and generates an electric field around 3 MV/cm.
Piezoelectric polarization The piezoelectric polarization is, as its name in-dicates, explained by the piezoelectric effect : because of the lattice mismatch between the AlGaN and GaN layers, the resulting mechanical constraint induces and electric field of around 2 MV/cm. This value is influenced by the Al percen-tage and thus the induced deformation in the crystalline structure. The vectorial sum between both types of polarization in the AlGaN/GaN heterostructure results in the apparition of positive fixed charges at the interface on the AlGaN side, as shown in figure1.9 :
1.2. PLACE OF GAN IN POWER ELECTRONICS 23
Supposing GaN is not constrained, it is possible to precisely calculate the sur-facic charge density that is generated depending of the x in AlxGa1−x  :
|σ(x)| = |PP E(AlxGa1−xN ) + PSP(AlxGa1−xN ) − PSP(GaN )| (1.10)
|σ(x)| = |2a(0) − a(x)
a(x) (e31(x) − e33(x)
) + PSP(x) − PSP(0)| (1.11)
with : - the lattice constant a(x) = (-0.077x + 3.189)10−10 m - elastic constants C13(x) = (5x + 103) GPa and C33(x) = (-32x + 405) GPa - piezoelectric constants
e13(x) = (-0.11x - 4.49) C.m−2 and e33(x) = (0.73x - 0.73) C.m−2 - spontaneous
polarization PSP(x) = (-0.052x - 0.029)C.m−2
The electric field resulting from these positive charges will induce the accumu-lation of compensatory mobile negative charges, the electrons, at the interface on the GaN side. As a consequence, we can deduce that the maximum theoretical electron density in the channel will be limited by the polarization charge density σ(x) (assuming all the charges are compensated).
Using non-doped semiconductors combined with the quantum confinement phe-nomenon will reduce electronic interactions in order to maintain maximum electron mobility in the channel (2000 cm−2/V.s) highly superior to the mobility in doped bulk GaN. There resides all the HEMT interest for microwave applications.
18.104.22.168 Bidimensional electron channel
The 2D electron gas is located in the GaN region of the AlGaN/GaN interface. As stated earlier, it is achieved through the heterojunction between AlGaN and GaN, giving birth to a high surface density of electrons. The density of carriers in the 2DEG is subject to changes depending on the growth conditions, namely the Al content. The best way to increase it is to put more aluminum in the AlGaN
barrier layer. However, beyond 30% of Al, the channel resistance increases signifi-cantly due to a diffusion of the alloy or interface roughness. Furthermore, the gate leakage current may increase as well with the Al concentration, which could lead to premature gate breakdown. The introduction of an AlN layer between AlGaN and GaN can counterbalance those effects , but will also generate instabilities at the gate contact level. It has indeed been reported that gate transistor with an AlN layer is unstable through direct polarization after a current stress of 5 mA/mm, whereas AlN free transistors were able to sustain 100 mA/mm without instability . Those perturbations are attributed to a high barrier height sen-sibility regarding the AlN thickness. A little variation of the AlN thickness may generate high currents locally when a small direct polarization is applied to the gate. The control of the AlN layer is thus capital if we want to achieve reliable structures for power devices.
The creation of an electron channel in the GaN layer is due to the forma-tion of a potential well at the AlGaN/GaN interface. In order to understand his phenomenon, it is necessary to study the band structure at the AlGaN/GaN he-terojunction. At the junction of 2 semiconductors, an electron diffusion will take place and, because of the difference in electronic affinity between the 2 materials, the electrons in AlGaN have a larger potential energy than those in GaN. The free electrons in AlGaN will thus spread towards GaN and accumulate at the interface. This diffusion will stop once thermodynamical equilibrium is achieved, that is to say when the Fermi levels of both materials are aligned.
EF AlGaN = EF GaN (1.12)
As shown in figure 1.10, a discontinuity of the conduction band and the Al-GaN/GaN interface appears and provokes the formation of a triangular potential well in GaN because of the band curving, with or without achieving the equili-brium state. Carriers will then accumulate in this well and will be responsible for the conduction phenomenon in the transistor. Since they are confined on a very
1.2. PLACE OF GAN IN POWER ELECTRONICS 25
small thickness, the electrons will form the so-called 2D electron gas which is the transistor’s channel. Under the influence of an electric field, electrons will transit through this channel from the source to the drain of the transistor.
Cette discontinuité de la bande de conduction représente 70 % de la différence de largeur de
Figure 1.10 – AlGaN/GaN heterojunction.
Once the device is realized, the transistor effect will be assured by the Schottky gate contact : by applying a negative voltage on the gate, the space charge region at the metal/semiconductor junction will rise, and beyond a certain value, a di-minution of the electrons concentration in the channel will occur. The transistor presents a "Normally-ON" behavior, which means it conducts current when no gate voltage is applied.
The discontinuity in the conduction band represents around 70% of the forbid-den gap energy difference between the 2 materials and is directly related to the aluminum content of the AlGaN layer .
∆EC = 0.7[Eg(x) − Eg(0) (1.13)
Eg(x) = x · Eg(AlN ) + (1 − x) · Eg(GaN ) − x · (1 − x)1.0eV s (1.14)
Models and formation mechanisms
While it is admitted that this electrical compensation phenomenon is at the origin of the 2D electron gas formation, its creation mechanisms are still poorly known, especially when it comes to the origin of the electrons. The most commonly ad-mitted hypothesis is of a high charge density at the AlGaN barrier surface which neutralizes polarization charges and is the source of the electron gas. Multiple stu-dies have been conducted in order to determine the natures of those surface states and different models have been investigated.
First model : single donor level In this particular model, we only consider one state of surface energy ED below the conduction band . This state is considered
as a donor state : electrically neutral when occupied, and positively charged when it has lost its electron. If the level is deep enough, it will be positioned initially under the Fermi level and the 2D gas will be empty : nSU RF = nS = 0 (nS being
the surface charge density in the 2DEG). While increasing the barrier thickness, the surface potential will rise due to the constant polarization electric field. Upon reaching a critical thickness tCR, the donor level will reach the Fermi level and
electrons will start to migrate from the occupied states of the surface to the empty states in the well in order to create the 2DEG. Upon doing so, the positive surface states will compensate the negative polarization charges at the surface and the electrons in the 2DEG will neutralize the positive charges at the interface. As long as all the surface states are not empty, the surface barrier height remains constant (EF = ED). This is what is called "Fermi level pinning" and is illustrated in figure
1.11. More electrons will migrate when the AlGaN increases and as such, the global electric field will tend to decrease.
1.2. PLACE OF GAN IN POWER ELECTRONICS 27
Figure 1.11 – Energy diagram of the AlGaN/GaN illustrating the one donor surface level model where the AlGaN thickness is (a) inferior and (b) superior to the critical thickness. (c) is the 2D electron density calculation depending on the AlGaN barrier thickness, for a one donor level model .
The Poisson equation allows to calculate the critical thickness tCR :
(ED − ∆EC) ·
q · σ (1.16)
where q is the elementary charge and σ the polarization charges.
Supposing every electron coming form the AlGaN surface compensates a pola-rization charge at the AlGaN/GaN interface, we can deduce the following relation :
Q = σ − nS (1.17)
with Q the polarization charges which are not compensated by the electrons contri-buting to the electric field.
But since the electric field is directly related to the sum of the electric charges at the interface, we can precisely calculate the electron density of the 2DEG
de-pending on the AlGaN electric field and the layer’s thickness : nS = σ q − dq2(ED + EF − ∆EC) (1.18)
where d is the AlGaN barrier thickness and EF the Fermi energy given by  :
EF = E0 +
m∗ nS (1.19)
where E0 is the energy of the first level formed in the quantum well between the
2 semiconductors : E0 = ( 9πhq2 80 √ 8m∗ ns ) 2/3 (1.20)
If we neglect the rise of the Fermi level in the channel, the 2DEG becomes :
qnS = σ(1 −
t ) (1.21)
As we can see in figure1.12, the density measurements done by Hall effect (black dots) tend to confirm the theory for low thicknesses. We can see the apparition of the 2DEG at 35 Å which allows us to estimate the surface donor energy at ED = 1.65 eV. The fall of the nS after 150Å can presuppose a relaxation of the
constraints in AlGaN for superior thicknesses.
Figure 1.12 – Room temperature 2DEG density measured by Hall effect as a function of Al0.34Ga0.64N barrier thickness .
1.2. PLACE OF GAN IN POWER ELECTRONICS 29
Theoretically, there is a saturation of the 2D electron gas density for important AlGaN thicknesses. The electric field at the interface will tend to decrease as long as the thickness increases, and will become null when all the polarization charges are neutralized. This explains the asymptotic behavior.
Second model : donor state distribution at the surface Even if the pre-vious model works well, it has been contradicted by multiple studies [17, 18], particularly regarding the surface barrier height at the AlGaN barrier. The publi-shed results that we can see in figure 1.13 indeed showed that the surface barrier height decreases when the AlGaN thickness rises, which is incompatible with the one donor state model.
FIG. 1. The bare surface barrier heights, obtained by simulation using the
Figure 1.13 – Variation of the AlGaN surface barrier height depending on the AlGaN layer thickness 
Starting from this observation, we can assume that the surface states are dis-tributed in the material gap. We thus consider a critical barrier height ΦC
(poten-tial between the conduction band and the highest occupied surface state) and a constant surface states density n0. Upon increasing the barrier thickness and if n0
is low enough, the barrier height at the surface will necessarily increase in order to allow the transition of more electrons to the 2DEG. All the surface states which
height is inferior to the barrier’s ΦS will as such contribute to the formation of the
2DEG by losing their electron, as shown in figure1.14and the following equation :
nSU RF = nS = n0(ΦS− ΦC) (1.22)
Figure 1.14 – Energy for the AlGaN/GaN heterostructure illustrating the electron transfer between the surface states and the 2DEG at the AlGaN/GaN interface .
This model is very close to the previous one, except that the barrier height ΦS is modified with the AlGaN thickness. The formula for the electron density
in the 2DEG is similar, but the donor state energy ED is replaced by the surface
potential ΦS, giving the following equation :
da2(ΦS+ EF − ∆EC) (1.23)
The variations of ΦS in function of the thickness d are directly related to the
states density n0 : the lower n0 is, the more important the variations of ΦS will be.
If the states density of surface donors is high enough, the electrons transfer from the surface to the 2DEG will only have a slight influence on the Fermi level. As
1.3. CONTEXT OF PH.D. 31
such, we are in the same configuration as in the first model with only one donor state, assuming the hypothesis that ED = qΦC and that the surface states density
However, multiple studies have shown noticeable differences regarding n0, ΦC
and ∆Φ (barrier height elevation) of the measured donor states at the surface, as can be seen in table 1.7. Those variations can be attributed to the different experience conditions, particularly if we take AlGaN oxides into account. Different studies [20, 21] have shown that oxidation has an influence on the surface proper-ties. Depending on the type of reconstruction with the oxygen atoms, the state density as well as the energy levels of the highest occupied state are modified, and this will have a direct influence on the formation of the 2D electron gas.
Source n0 (cm−2.eV−1) ΦC (eV) ∆Φ (eV)
Ibbeston et al. ∞ 1.65 0
Koley et al. 1.6 x1013 1.0 0.8
Higashiwaki et al. 4 - 6 x 1012 1.0 1.5
Gordon et al. <1013 1.0 1.3
Table 1.7 – Parameters differences between different studies
Context of Ph.D.
As stated at the beginning of this work, the demand regarding power devices is in a large expansion and is expected to expand even further in the years to come. Compared to the silicon industry, gallium-nitride technology is still at its beginning and what we know so far about it is probably just the tip of the iceberg. However, in an energy driven economical context, the HEMT structure represents a very promising solution for achieving high power and frequency switching devices. But even though theory predicts high performances for AlGaN/GaN heterostructures, we are still very dependent on material quality and process steps. As stated earlier, GaN epitaxy is complicated, and there are still a lot of problems preventing us for
achieving performances as high as we would like. Whether it be defects, doping or device architecture challenges, every step in the elaboration process brings its fair share of difficulties, and each one of them must be addressed separately.
This works takes place in the context of the creation of GaN on silicon industry oriented device processing chain in the LC2E laboratory. Using the already present CMOS industry equipment of the CEA-Leti, the objective here is to achieve high performance devices for power applications with cost reduction through the use of large diameter 200 mm silicon substrates.
In terms of device technology and considering its maturity on silicon, the Schottky gate structure has been studied intensively and already yielded some good results. However, for it to be reliable, a very good control of the different creation processes is necessary. Even though it has proven to be a very robust structure, it still presents some defects, particularly in terms of gate leakage cur-rent, and its performances are very sensitive to material quality. The natural way to reduce this hindrance would be, as in the silicon industry, to turn to the use of an intermediate insulating layer between the gate and the material to achieve MOS-like devices.
This is precisely where this work will be integrated. From the choice of the insulator to its electrical testing, going through deposition, characterization, pre-or post-processing and material conditioning, it was my wpre-ork as a Ph.D student in CEA-Leti to address the different challenges in order to create a reliable MIS-HEMT device (MIS standing for Metal Insulator Semiconductor). Most of the research was carried on wafers produced at CEA-Leti, but also on some samples coming from the III-V Lab in Paris.
The main objective in the elaboration of a MIS-HEMT during my work was to address one of the major problematic in power device elaboration, which is to suppress or at least greatly reduce the gate-leakage current. As the continuous down-scaling of the device size has lead to very thin gate oxides, the leakage current that can flow from the channel to the gate comes into the order of the subthreshold
1.4. CONCLUSION 33
leakage current and the gate cannot be considered as an ideally insulated electrode anymore. This affects the circuit functionality and increases the standby power consumption due to the static gate current. Another key aspect directly following, is to elaborate a sufficiently robust and optimal process in order to better achieve a normally-off device. Ultimately, and mainly for safety reasons, it is preferable to apply a positive gate bias in order to open the device channel, instead of applying a negative bias in order to close it.
While introducing a gate dielectric is a very good solution towards solving the above mentioned problems, it also comes with its limitations and constraints typically found in CMOS structures in general. As we will see in the next chapter, we also have to take into account the potential barrier height of the dielectric and the critical electric field.
In this first chapter, we first analyzed what are the present and future demands regarding the market for power devices and their applications. That led to the conclusion that silicon has now reached its limits in order for it to stay competitive in those domains of applications and the necessity to switch to large band gap materials.
As such, we have seen that gallium nitride has a place of choice among such materials and enunciated the different properties, showings its particular place in the microelectronics industry. Among the two different forms, we have seen that the hexagonal structure presents many advantages over the cubic one. The different advantages of the use of GaN over conventional semiconductors for power and high frequency switching applications were then exposed, and the AlGaN/GaN heterostructure was introduced. This showed the particularly interesting 2DEG generation for the elaboration of HEMT devices.
of GaN. Even if great progress has been made in recent years, it still appears that it is too complex and expensive to produce bulk GaN, but hetero-epitaxy through MOCVD on silicon is making great progress, allowing the creation of large diameter GaN production chain at high quality levels, despite the still large quantity of defects generated.
Lastly, a brief introduction of this Ph.D. subject was enunciated in order to emphasize the importance of GaN and its properties in the elaboration of MIS-HEMT structures.
The Metal Insulator Semiconductor
structure on GaN
Presentation of the structure
Principle of operation
The first structures using two dimension electron gas appeared in 1980 and were created by Thomson-CSF  and Fujitsu  under the form of MESFETs (MEtal Semiconductor Field Effect Transistor) which used doped gallium arsenide GaAs. These simple structures were later on replaced by HEMT in the mid 90s , using AlGaAs/GaAs and AlGaAs/InGaAs heterostructures. Due to the presence
of the two dimensional electron gas at the AlGaN/GaN interface, these structure have also been labelled as TEGFETs (Two dimensional Electron Gas Field Effect Transistors).
As presented in the first chapter, the AlGaN/GaN heterostructure is the solu-tion envisioned in order to realize reliable power devices on GaN. In order to take maximum advantage of the high mobility of the electrons and the high electric field, one of the first studied architecture for HEMT devices is the Schottky gate transistor.
Having a long history of development on silicon architectures, it has been well adapted to fit high power demands over the years. Figure 2.1 shows a typical Schottky gate structure for an AlGaN/GaN HEMT.
Figure 2.1 – Schematics of a Schottky gate transistor on an AlGaN/GaN hete-rostructure
As seen in chapter 1, the AlGaN layer’s gap is more important than the one of GaN (the difference is even more important with higher Al concentration). The gate is metallic and is the element making a Schottky contact with the semi-conductor. Once a high polarization is applied, the gate will deplete the electron channel locally, making the AlGaN layer an insulator. The electrons coming from the donors are then transferred to the non intentionally doped GaN, which will increase their density at the AlGaN/GaN interface (heterojunction) : this is what is called the channel and is only a few nanometers thick. In this region, electron mobility is very high, because of the lack of donor ions in non intentionally doped GaN. The behavior of these carriers inside potential wells can be described through
2.1. PRESENTATION OF THE STRUCTURE 37
the use of quantum mechanics (Schrödinger-Poisson equations) which we will not detail here. The source and drain are metallic contacts and constitute what are called the ohmic contacts.
One important characteristic to point out is that those transistors function in a normally-on state. This means that the device is naturally in a conducting "on" state where the carriers can flow freely. In order to deplete the channel, it is thus necessary to apply a negative bias on the gate.
One of the major challenge to date is the finality of achieving normally-off devices. It is obvious that for security reasons, we need the power component to be in the off state when no bias is applied to the gate. Taking this into consideration, the MIS (Metal Insulator Semiconductor) structure represents a viable possibility because it allows positive gate bias without gate current injection, and reduces the gate leakage currents to a minimum whether it be in the open or closed state. The principle of the structure is to add an insulator layer between the metallic gate and the AlGaN barrier, as shown in figure 2.2.
Figure 2.2 – Schematics of a HEMT with insulated gate transistor on an Al-GaN/GaN heterostructure
The metal-semiconductor junction
22.214.171.124 Full depletion approximation
The simple analytic model of the metal-semiconductor junction is based on the full depletion approximation. This approximation is obtained by assuming that